General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.66 - 7.7 g/cm³ Show Material materials with Density of 7.66 - 7.7 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | 20.0 °C | 203 GPa Show Material materials with Elastic modulus of 203 GPa | |

100.0 °C | 197 GPa Show Material materials with Elastic modulus of 197 GPa | ||

200.0 °C | 190 GPa Show Material materials with Elastic modulus of 190 GPa | ||

300.0 °C | 181 GPa Show Material materials with Elastic modulus of 181 GPa | ||

400.0 °C | 171 GPa Show Material materials with Elastic modulus of 171 GPa | ||

500.0 °C | 158 GPa Show Material materials with Elastic modulus of 158 GPa | ||

600.0 °C | 147 GPa Show Material materials with Elastic modulus of 147 GPa | ||

700.0 °C | 140 GPa Show Material materials with Elastic modulus of 140 GPa | ||

800.0 °C | 135 GPa Show Material materials with Elastic modulus of 135 GPa | ||

900.0 °C | 131 GPa Show Material materials with Elastic modulus of 131 GPa | ||

1000.0 °C | 127 GPa Show Material materials with Elastic modulus of 127 GPa | ||

Elongation | 20.0 °C | 16 % Show Material materials with Elongation of 16 % | |

Elongation, transverse | 20.0 °C | 12 % Show Material materials with Elongation, transverse of 12 % | |

Hardness, Brinell | 20.0 °C | 235 [-] Show Material materials with Hardness, Brinell of 235 [-] | |

Poisson's ratio | 23.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | Typical for Austenitic Stainless Steel |

Shear modulus | 23.0 °C | 77 GPa Show Material materials with Shear modulus of 77 GPa | Typical for Austenitic Stainless Steel |

Tensile strength | 20.0 °C | 600 - 850 MPa Show Material materials with Tensile strength of 600 - 850 MPa | |

Tensile strength, transverse | 20.0 °C | 600 - 850 MPa Show Material materials with Tensile strength, transverse of 600 - 850 MPa | |

Yield strength Rp0.2 | 20.0 °C | 400 MPa Show Material materials with Yield strength Rp0.2 of 400 MPa | |

Yield strength Rp0.2, transverse | 20.0 °C | 400 MPa Show Material materials with Yield strength Rp0.2, transverse of 400 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.08E-5 1/K | |

20.0 °C | 1.15E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.15E-5 1/K | ||

100.0 °C | 1.18E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.18E-5 1/K | ||

200.0 °C | 1.24E-5 - 1.3E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.24E-5 - 1.3E-5 1/K | ||

300.0 °C | 1.29E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.29E-5 1/K | ||

400.0 °C | 1.32E-5 - 1.35E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.32E-5 - 1.35E-5 1/K | ||

500.0 °C | 1.35E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.35E-5 1/K | ||

600.0 °C | 1.38E-5 - 1.4E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.38E-5 - 1.4E-5 1/K | ||

700.0 °C | 1.4E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.4E-5 1/K | ||

800.0 °C | 1.42E-5 - 1.45E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.42E-5 - 1.45E-5 1/K | ||

900.0 °C | 1.46E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.46E-5 1/K | ||

1000.0 °C | 1.48E-5 - 1.5E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.48E-5 - 1.5E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | 0 - 950 °C Show Material materials with Max service temperature, long of 0 - 950 °C | ||

Melting point | 1230 - 1480 °C Show Material materials with Melting point of 1230 - 1480 °C | Typical for Austenitic Stainless Steel | |

Specific heat capacity | 20.0 °C | 459 - 500 J/(kg·K) Show Material materials with Specific heat capacity of 459 - 500 J/(kg·K) | |

100.0 °C | 498 J/(kg·K) Show Material materials with Specific heat capacity of 498 J/(kg·K) | ||

200.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

300.0 °C | 549 J/(kg·K) Show Material materials with Specific heat capacity of 549 J/(kg·K) | ||

400.0 °C | 569 J/(kg·K) Show Material materials with Specific heat capacity of 569 J/(kg·K) | ||

500.0 °C | 594 J/(kg·K) Show Material materials with Specific heat capacity of 594 J/(kg·K) | ||

600.0 °C | 632 J/(kg·K) Show Material materials with Specific heat capacity of 632 J/(kg·K) | ||

700.0 °C | 640 J/(kg·K) Show Material materials with Specific heat capacity of 640 J/(kg·K) | ||

800.0 °C | 642 J/(kg·K) Show Material materials with Specific heat capacity of 642 J/(kg·K) | ||

900.0 °C | 643 J/(kg·K) Show Material materials with Specific heat capacity of 643 J/(kg·K) | ||

1000.0 °C | 645 J/(kg·K) Show Material materials with Specific heat capacity of 645 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 17 - 17.2 W/(m·K) Show Material materials with Thermal conductivity of 17 - 17.2 W/(m·K) | |

100.0 °C | 18.3 W/(m·K) Show Material materials with Thermal conductivity of 18.3 W/(m·K) | ||

200.0 °C | 19.5 W/(m·K) Show Material materials with Thermal conductivity of 19.5 W/(m·K) | ||

300.0 °C | 20.8 W/(m·K) Show Material materials with Thermal conductivity of 20.8 W/(m·K) | ||

400.0 °C | 21.8 W/(m·K) Show Material materials with Thermal conductivity of 21.8 W/(m·K) | ||

500.0 °C | 22.7 - 23 W/(m·K) Show Material materials with Thermal conductivity of 22.7 - 23 W/(m·K) | ||

600.0 °C | 23.6 W/(m·K) Show Material materials with Thermal conductivity of 23.6 W/(m·K) | ||

700.0 °C | 24.9 W/(m·K) Show Material materials with Thermal conductivity of 24.9 W/(m·K) | ||

800.0 °C | 26.1 W/(m·K) Show Material materials with Thermal conductivity of 26.1 W/(m·K) | ||

900.0 °C | 27.6 W/(m·K) Show Material materials with Thermal conductivity of 27.6 W/(m·K) | ||

1000.0 °C | 28.8 W/(m·K) Show Material materials with Thermal conductivity of 28.8 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 4.9 mm²/s Show Material materials with Thermal diffusivity of 4.9 mm²/s | |

100.0 °C | 4.5 mm²/s Show Material materials with Thermal diffusivity of 4.5 mm²/s | ||

200.0 °C | 4.5 mm²/s Show Material materials with Thermal diffusivity of 4.5 mm²/s | ||

300.0 °C | 4.6 mm²/s Show Material materials with Thermal diffusivity of 4.6 mm²/s | ||

400.0 °C | 4.6 mm²/s Show Material materials with Thermal diffusivity of 4.6 mm²/s | ||

500.0 °C | 3.6 mm²/s Show Material materials with Thermal diffusivity of 3.6 mm²/s | ||

600.0 °C | 4.2 mm²/s Show Material materials with Thermal diffusivity of 4.2 mm²/s | ||

700.0 °C | 5.1 mm²/s Show Material materials with Thermal diffusivity of 5.1 mm²/s | ||

800.0 °C | 5.4 mm²/s Show Material materials with Thermal diffusivity of 5.4 mm²/s | ||

900.0 °C | 5.7 mm²/s Show Material materials with Thermal diffusivity of 5.7 mm²/s | ||

1000.0 °C | 5.9 mm²/s Show Material materials with Thermal diffusivity of 5.9 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 8.41E-7 - 9E-7 Ω·m Show Material materials with Electrical resistivity of 8.41E-7 - 9E-7 Ω·m |

100.0 °C | 8.89E-7 Ω·m Show Material materials with Electrical resistivity of 8.89E-7 Ω·m | |

200.0 °C | 9.47E-7 Ω·m Show Material materials with Electrical resistivity of 9.47E-7 Ω·m | |

300.0 °C | 9.91E-7 Ω·m Show Material materials with Electrical resistivity of 9.91E-7 Ω·m | |

400.0 °C | 1.05E-6 Ω·m Show Material materials with Electrical resistivity of 1.05E-6 Ω·m | |

500.0 °C | 1.1E-6 Ω·m Show Material materials with Electrical resistivity of 1.1E-6 Ω·m | |

600.0 °C | 1.15E-6 Ω·m Show Material materials with Electrical resistivity of 1.15E-6 Ω·m | |

700.0 °C | 1.18E-6 Ω·m Show Material materials with Electrical resistivity of 1.18E-6 Ω·m | |

800.0 °C | 1.21E-6 Ω·m Show Material materials with Electrical resistivity of 1.21E-6 Ω·m | |

900.0 °C | 1.23E-6 Ω·m Show Material materials with Electrical resistivity of 1.23E-6 Ω·m | |

1000.0 °C | 1.25E-6 Ω·m Show Material materials with Electrical resistivity of 1.25E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.1 - 0.2 % Show Material materials with Carbon of 0.1 - 0.2 % |

Chromium | 24.5 - 26.5 % Show Material materials with Chromium of 24.5 - 26.5 % |

Manganese | 2 % Show Material materials with Manganese of 2 % |

Nickel | 3.5 - 5.5 % Show Material materials with Nickel of 3.5 - 5.5 % |

Nitrogen | 0.11 % Show Material materials with Nitrogen of 0.11 % |

Phosphorus | 0.04 % Show Material materials with Phosphorus of 0.04 % |

Silicon | 0.8 - 1.5 % Show Material materials with Silicon of 0.8 - 1.5 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |